DOI: 10.5281/zenodo.15527838
title: INR18650-LG-3500-MJ1 Anode GITT Overpotential

description: Scope

This record contains overpotential observed in GITT measurements during discharge and charge, pre-selected and packaged in parquet files for further analysis.The GITT measurements were obtained from negative electrode (anode) harvested from an INR18650-MJ1 Li-ion battery cell manufactured by LG CHEM. The active material in the electrode is composite graphite/silicon oxide. The measurment is obtained in three-electrode configuration with the working electrode composite graphite/silicon oxide, counter electrode NMC, and reference electrode lithium metal in a coin cell casing.

Files

Data




Filename
Description
Format
Usage




18650-LG-3500-MJ1-Anode GITT_dch ohne EIS(2320)_overpotential.parquet
Parquet file containing overpotential data extracted from GITT discharge tests without EIS (ID: 2320).
Parquet (application/octet-stream)
Used for detailed analysis and modeling of GITT discharge overpotential behavior.


18650-LG-3500-MJ1-Anode GITT_ch ohne EIS(2340)_overpotential.parquet
Parquet file containing overpotential data extracted from GITT charge tests without EIS (ID: 2340).
Parquet (application/octet-stream)
Supports detailed analysis of charge overpotential data for battery performance studies.




Plots




Filename
Description
Format
Usage




18650-LG-3500-MJ1-Anode GITT_dch ohne EIS(2320)_extraction_with_negative_soc_ocv_alignment.pdf
PDF document summarizing OCV alignment and negative SOC extraction for GITT discharge data (ID: 2320).
PDF (application/pdf)
Provides visualized summary of OCV alignment and data extraction processes.


18650-LG-3500-MJ1-Anode GITT_ch ohne EIS(2340)_extraction_with_negative_soc_ocv_alignment.pdf
PDF document summarizing OCV alignment and negative SOC extraction for GITT charge data (ID: 2340).
PDF (application/pdf)
Used for reporting on GITT charge data with SOC alignment processes.




Related Resources




Relationship
Record
Description


isPartOf
INR18650-LG-3500-MJ1 Anode
This collection points to all the intermediate steps including and between the data obtained on the harvested anode of the MJ1 cylindrical 18650 cell from LG CHEM and its analysis.


Continues
INR18650-LG-3500-MJ1 Anode GITT Structured Data


This record contains GITT measurements during discharge and charge, pre-selected and packaged in parquet files for further analysis. The measurement is obtained in three-electrode configuration with the working electrode composite graphite/silicon oxide, counter electrode NMC, and reference electrode lithium metal in a coin cell casing. The data is intended to support the characterization of the open-circuit potential (OCP) and lithium diffusion proprties of the graphite/silicon oxide active material.

 



Continues
INR18650-LG-3500-MJ1 Anode GITT OCV
This record contains open-circuit voltage (OCV) data extracted from a GITT measurement on the harvested anode of the MJ1 cylindrical 18650 cell from LG CHEM. The active material of the harvested electrode is composite graphite/silicon oxide. The measurment is obtained in three-electrode configuration with the working electrode composite graphite/silicon oxide, counter electrode NMC, and reference electrode lithium metal in a coin cell casing. The data is intended to support the generation of parameterized OCV curves for use in battery cell modelling.


Continues
INR18650-LG-3500-MJ1 Anode GITT Overpotential Extraction
This record contains workflows that extracts the cell overpotential from GITT measurements during discharging and charging.


IsContinuedBy
18650-LG-3500-MJ1 Anode GITT Featurization
This record contains workflows to extract feactures from the GITT (without intermittent EIS) measurement on the harvested negative electrode (anode) of the INR18650-MJ1 Li-ion battery cell from LG CHEM. It simulteaneously sets up the simulator and EP-BOLFI optimizer inputs for later parameterization.




Metadata

Machine Readable RDF




Filename
Description
Format
Usage




Human Readable Tables

Working Electrode




Property
Value




Comment
Harvested from INR18650-MJ1


Active Material 1
Graphite


Active Material 1 Volume Fraction / 1
0.965


Active Material 2
Silicon Oxide


Active Material 2 Volume Fraction / 1
0.035


Active Material Composite Lithium Saturation Concentration / mol L-1
29.254


Electrode Thickness / µm
87




Counter Electrode




Property
Value




Comment
Harvested from INR18650-MJ1


Active Material
NCM-831205


Active Material Molecular Formula
LiNi0.83Co0.12Mn0.05O2


Electrode Thickness / µm
73




Reference Electrode




Property
Value




Comment
Lithium Metal


Active Material
Lithium




Separator




Property
Value




Type
Whatman GF/A


Supplier
El-cell


Thickness / µm
260


Porosity
0.93




Electrolyte




Property
Value




Type
1M LiPF6 in EC:EMC:DMC 1:1:1


Salt
LiPF6


Salt Concentration / mol L-1
1


Solvent 1
Ethylene Carbonate


Solvent 2
Ethyl Methyl Carbonate


Solvent 3
Dimethyl Carbonate




Cell




Property
Value




Format
Coin Cell


Dimensions
R2032


Nominal Capacity / mAh
12




Licensing

This dataset is licensed under CC-BY 4.0, allowing for sharing and adaptation with proper attribution.

Contact Information

For questions or further assistance, please contact Dennis Kopljar at dennis.kopljar@dlr.de.

References

This dataset is linked to the following publication: [DOI/Link to publication].